\YOOD-! -sl.\(i IN'nrSTKIFS OF CALIFORNIA. 75 



Spanish cedar. Mexico. 



Of total amount of Spanish cedar i Manufactured 0.9 per cent used in 

 this industry. 



Balusters; newels MI id rails on stairs. 



Turns well ; good finish. 



Rough, clear, 1 to 6 inches thick. 



Eastern ash (white ash). Middle West; South. 



Of total amount of eastern ash manufactured 0.8 per cent used in this 

 industry. 



Cabinet work. 



Rough, clear and select, 1 to 4 inches thick. 



Australian blue gum. Australia. 



Of total amount of Australian blue gum manufactured 32.3 per cent 

 used in this industry. 



Turnings. 



Boards, planks, blocks, 1 to 6 inches thick. 



Oregon maple. Oregon. 



Of total amount of Oregon maple manufactured 14.6 per. cent used in 

 this industry. 



Mantels. 



Good finish. 



Rough, first grade, 1 to 4 inches thick. 



Genisaro (Jenizaro). Mexico. 



Of total amount of Genisaro manufactured 1.1 per cent used in this 

 industry. 



Cabinet work ; stairs. 



Rough, clear and select, 1 to 4 inches thick. 



Yellow poplar (whitewood). Middle West; South. 



Of total amount of yellow poplar manufactured 0.4 per cent used in 

 this industry. 



Cabinet work ; carved work ; mantels. 



Works easily ; good finish. 



( 'abinet work : surfaced on two sides, clear, \ inch thick. 



Mantels : rough, first grade, 1 to 2 inches thick. 



Pepperwood (California laurel). California. 



Of total amount of pepperwood manufactured 30.7 per cent used in 

 tliis industry. 



( 'abinet work ; mantels. 



Strong; good finish. 



Cabinet work : rough, No. 1 and 2, 1 to 6 inches thick. 



Mantels : No. 1, 1^ inches thick. 



